### SlideShare for iOS

by Linkedin Corporation

FREE - On the App Store

- Total Views
- 218
- Views on SlideShare
- 218
- Embed Views

- Likes
- 0
- Downloads
- 1
- Comments
- 0

No embeds

Uploaded via SlideShare as Adobe PDF

© All Rights Reserved

- 1. R.Umamaheswara rao, S.Santhosh Kumar, M.Santhi Kumar / International Journal of Engineering Research and Applications (IJERA) ISSN: 2248-9622 www.ijera.com Vol. 2, Issue4, July-August 2012, pp.1451-1458 Preparation And Characterization Of Polymer Nanocomposites For Damping. R.Umamaheswara rao1, S.Santhosh Kumar2, M.Santhi Kumar3. (Department of Mechanical Engineering, GMR Institute of Technology, Rajam-532127. Srikakulam District, Andhra Pradesh, INDIA.ABSTRACT Carbon nanotube-based composite is damping holds the potential for improving Trackingbecoming increasingly popular and offers great and positioning characteristics such as those of apotential for highly demanding practical high read/write head of a computer hard disk drive and thestrength and high damping applications. The accuracy of the weapon systems mounted on aircraftsexcellent damping capacity of CNTs is primarily and land systems. Other applications of dampingdue to the interfacial friction between carbon enhancement range from turbo-machinery andnanotubes and polymer resins and the extremely engine/equipment mounts to suspension and steeringlarge interfacial surface area over a given specific systems in automotive engineering. Therefore, it ismass (specific area). In this work pure MWCNT necessary to develop structural components with highwere used to blend with PLA and composite was level of mechanical damping for a wide variety ofprepared by melt-mixing under different CNT applications in aerospace, mechanical and civilloadings. Especially we concentrated on Dynamic engineering systems. Viscoelastic materials such ascharacterization of the nanocomposite. Dynamic high loss factor polymers have been the mostcharacterization is done by using DMA in which frequently used in modern damping applications [1–loss modulus, storage modulus and damping loss 5]. Elastomeric materials operated in simple shearfactor variations were determined with respect to were investigated both experimentally andfrequency. We interpreted DMA conditions in analytically and were used for helicopter damperANSYS and found amplitude which is input for applications [6]. Performance characteristics oftheoretical model based on interfacial friction magnetic constrained layer damping had beenbetween the PLA and MWCNT. The model, investigated by Baz and Poh [7]. Vibration/shockdeveloped is analytical and relates explicitly the absorbers were developed for automotive suspensionmaterial properties of the resin (PLA) and applications using electro-rheological fluids bynanotubes and the processing parameters to the Lindler and Wereley [8]. On the other hand, dampingoverall material damping loss factor and hence it properties of magneto-rheological fluids wereoffers the possibility for material engineers to investigated by Kamath et al. [9] and dampers forpossibly optimize the damping for required helicopter rotor blade applications were developed.applications. Using a passive capacitive shunt circuit, tunable solid- state piezoelectric vibration absorbers have beenKeywords - vibration of nanotubes, vibration investigated and developed for general aerospacedamping, damping of nanotubes, nanocomposite applications [10]. Recent research effort in thisDamping of nanocomposite, vibration of direction has been much focused on the developmentnanocomposite of polymer damping materials based on nanocomposites in which nanotubes, nanofibers or1. INTRODUCTION nanoparticles are embedded in polymer substrates and With the advances in technology and the much promising results have been established.increase in the global population, plastic materials Nanocomposites with embedded carbon nanotubeshave found wide applications in every aspect of life have recently been rigorously pursued for their superband industries. However, most plastics such as mechanical strength as well as their potential dampingpolyethylene, polypropylene, and polystyrene are non capacities [11–13]. In addition, other types ofbiodegradable, and their increasing accumulation in nanocomposites have also been investigated such asthe environment has been a threat to the planet. To those modified with nanoclay [14–15] and have beenovercome all these problems, some steps have been found effective for damping applications. This report,undertaken.PLA, though discovered, & Enhancement however, will focus on the modeling of dampingof damping in a structural system can lead to mechanism of carbon nanotube-basedalleviation of aero elastic flutter, reduction of gust nanocomposites. which is used for converting nonloading, increased fatigue life of structural linear spring characteristics to linear form. Bycomponents, improved cabin noise, maneuverability conducting harmonic analysis in ANSYS we foundand handling. In fact, high structural damping is an the amplitudes for the testing specimen and theseImportant design parameter for all machine elements amplitudes were used as inputs for the mathematicaland manufacturing tools. In addition, enhancement of model. 1451 | P a g e
- 2. R.Umamaheswara rao, S.Santhosh Kumar, M.Santhi Kumar / International Journal of Engineering Research and Applications (IJERA) ISSN: 2248-9622 www.ijera.com Vol. 2, Issue4, July-August 2012, pp.1451-14582. MELT BLENDING 3.2. PRINCIPLE OF DMA:2.1. Processing of PLA with MWCNT: Dynamic mechanical analysis (DMA) yieldsPrior to processing, PLA was dried in an oven set at information about the mechanical properties of a55ºC for four hours to remove any absorbed specimen placed in minor, usually sinusoidal,moisture.PLA is blended with MWCNT in the oscillation as a function of time and temperature byfollowing four different proportions. subjecting it to a small, usually sinusoidal, oscillating» PLA + 0.2 wt% MWCNT force. The applied mechanical load, that is, stress,» PLA + 0.5 wt% MWCNT elicits a corresponding strain (deformation) whose» PLA + 1.0 wt% MWCNT amplitude and phase shift can be determined.» PLA + 2.0 wt% MWCNTFinally, the PLA and MWCNT neat resin were 3.3. TESTING MODE:extruded using a 32-mm (L/D = 20) Davis Standardco-rotating twin extruder at a temperature of 170ºCwith 6 minutes duration at 50 rpm speed to create apolymer matrix of PLA and MWCNT of fourdifferent proportions mentioned above. The twinscrew extruder was configured with mixing elementsthat were capable of providing additional shear. Theextruded material then was chopped into small pelletsusing a pelletizer2.2. COMPRESSION MOLDING: Compression molding is a method of Figure 1: Single Cantilever modemolding in which the molding material, generally Specimen is clamped between the clamps aspreheated, is first placed in an open, heated mold shown in above figure as one end is fixed and at thecavity. The mold is closed with a top force or plug other end load is applied with a frequency range of 0-member, pressure is applied to force the material into 100 Hzcontact with all mold areas, while heat and pressureare maintained until the molding material has cured. 3.4. RESULTS FROM DMA:The process employs thermosetting resins in a 3.4.1. STORAGE MODULUS:partially cured stage, either in the form of granules, The storage modulus E´ represents theputty-like masses, or performs. Compression molding stiffness of a viscoelastic material and is proportionalis a high-volume, high-pressure method suitable for to the energy stored during a loading cycle. It ismolding complex, high-strength fiberglass roughly equal to the elastic modulus for a single, rapidreinforcements. Advanced composite thermoplastics stress at low load and reversible deformationcan also be compression molded with unidirectionaltapes, woven fabrics, randomly oriented fiber mat or 3.4.2. LOSS MODULUS:chopped strand. The advantage of compression The loss modulus E´´ is defined as beingmolding is its ability to mold large, fairly intricate proportional to the energy dissipated during oneparts.Also,it is one of the lowest cost molding loading cycle. It represents, for example, energy lostmethods compared with other methods such as as heat, and is a measure of vibrational energy thattransfer molding and injection molding; moreover it has been converted during vibration and that cannotwastes relatively little material, giving it an advantage be recovered.when working with expensive compound. However,compression molding often provides poor product 3.4.3. DAMPING LOSS FACTOR:consistency and difficulty in controlling flashing, and The loss factor tanδ is the ratio of lossit is not suitable for some type of parts. Compression modulus to storage modulus. It is a measure of themolding produces fewer knit lines and less fiber- energy lost, expressed in terms of the recoverablelength degradation than injection molding. According energy, and represents mechanical damping orto ASTM D1238, specimen size of 25x6x4 mm was internal friction in a viscoelastic system. The lossprepared by thread cutting factor tanδ is expressed as a dimensionless number. A high tanδ value is indicative of a material that has a high, nonelastic strain component, while a low value3. DMA (DYNAMIC MECHANICAL ANALYZER): indicates one that is more elastic.3.1. DMA-242CspecificationsTemperature range=150-600degCFrequency range=0.01-200Hz 4. THEORETICAL MODELINGForce range=0.0001-18N This mathematical modeling is based on the interfacial friction losses between the nanotubes, 1452 | P a g e
- 3. R.Umamaheswara rao, S.Santhosh Kumar, M.Santhi Kumar / International Journal of Engineering Research and Applications (IJERA) ISSN: 2248-9622 www.ijera.com Vol. 2, Issue4, July-August 2012, pp.1451-1458nanotubes and resin in the composite. This friction Stiffness of the outer layer (4)losses occurs due to shearing action of one layer over Where Er and En are the Young’s moduli of the resinanother while we apply load due to its viscoelastic and the nanotubes, respectively. Further assume thenature. critical stresses between the resin and the nanotubes and between the nanotubes at which slips occur to be4.1. Mathematical modeling: t1 and t2, and then interfacial friction limits can beDamping is physically an average measure of the rate written asof energy dissipation of a system. What are the major (5)energy dissipation mechanisms present in ananocomposite system with CNTs as reinforcements ( Is radius of the inner layer) (6)under cyclic loading? Three major sources can be The value of l can be selected as the typical length ofclearly identified and these are: (i) the inherent the nanotube reinforcement. The inertial forces duringmaterial damping of the base polymer, (ii) the vibration low frequencies can be neglected.frictional loss resulting from the slips between CNTs 4.2. Vibration analysis:and polymer resins and (iii), the frictional loss from Based on the basic cell element shown in Fig.10, onethe slips between CNTs themselves. Inherent material can derive its force-displacement relationships. Definedamping is 24 well understood and here we focus δ1=f1/k1, δ2=f2/k2 and assume δ1≤δ2, then when there isourselves on the understanding and modeling of the a displacement actuation input x=Asinѡt, the forcefrictional losses between CNTs and polymer resins output of the element can be established for the for theand between CNTs themselves. First, let us examine following actuation amplitude Aan ideal case where dispersed MWCNTs are 4.2.1. Interfacial slips between resin and nanotubesuniformly distributed among resins and are all ideally and nanotubes themselves:oriented along the axial direction as shown in Fig. When the input actuation amplitude becomes large (A≥δ2) both the interface between the resin and the nanotubes and that between the nanotubes themselves starts to slip and substantial friction loss will be generated leading to high level of mechanical damping capacity. The force-displacement relationship in this case can be shown in fig.Fig.2. Polymer with reinforced carbon nanotubes From vibration analysis point of view, such acell element can be modeled as a mass spring systemwith 3 springs representing the stiffness of the resin,the nano tube outer layer and the nano tube inner layeras shown in Fig.10. Here kR, k1 and k2 represent thestiffness and mR, m1 and m2 represent the masses ofthe resin, the outer layer of the carbon nanotubes andthe inner layers of the carbon nanotubes respectively.Therefore f1 and f2 represent the interfacial frictionlimits between the resin and the nanotubes andbetween the nanotubes at which slips between thesurfaces occur. These parameters of the model can bedetermined from the given material properties of theresin and the nanotubes such as Young’s modulus and Fig.4. Force-Displacement relationshipthe processing parameters such as volume fraction. It is first appropriate to examine this general case to see how a hysteretic loop is formed and hence energy dissipated during a vibration cycle. When x starts it increase but is less than δ1, the force- displacement relationship follows the line OP with an effective stiffness the sum of the three individual stiffness, K=K1+K2+Kr. Once it reaches P, k1 starts to slip. And the effective stiffness becomes K=Kr+K2Fig.3.Vibration analysis model of the basic cell until it gets to Q at which K2 also starts to slip. Henceelement from Q to R, the effective stiffness becomes K=K r. It then follows RS on its way back with no slip and thenVolumefraction (1) ST with K1 slipping and TU with both K1 and K2 isStiffness of the resin (2) slipping at the same time. Finally, it follows UV, VWStiffness of the outer layer (3) and WQ back to Q and a complete cycle under the 1453 | P a g e
- 4. R.Umamaheswara rao, S.Santhosh Kumar, M.Santhi Kumar / International Journal of Engineering Research and Applications (IJERA) ISSN: 2248-9622 www.ijera.com Vol. 2, Issue4, July-August 2012, pp.1451-1458sinusoidal displacement actuation. Having now defined as describing function N (A, w) underestablished the force-displacement relationship, from harmonic excitation.it one can derive the damping loss factor of the cell,which is also the damping loss factor of thenanocomposite material concerned. However, thesimple fact that the force-displacement relationshipinvolves a hysteretic loop implies that such a systemmodel is nonlinear with memory and someappropriate linearization procedure is required beforedamping loss factor of the system can be established.The most powerful and frequently used method,which can be employed to derive an accurateequivalent linearized model for a nonlinearcharacteristics shown in above fig. Describing Fig.5. Describing Functionfunction is used here to linearize the non linearcharacteristics.Sinusoidal input is (7)A and ѡ are constants and output can be expressed inFourier expression is (8)Where an and bn (n=1, 2, 3---) are real constants to bedetermined. The first two fundamental terms can bederived by multiplying both sides by andintegrating over [0,2п] with respect to as(9)(10)Here = (A, w) and b1=b1 (A, w), hence theoutput of first order approximation is(11)Using complex notation above equation can be Fig.6. input-output characteristics of the non linearwritten as force-displacement relationship. The sinusoidal input and the output of the nonlinearity can be sketched as shown in Fig.13. First, we need to establish the coordinates of points S and (12) W and with little analysis of the hysteresisNow we can define first order transfer function H1 characteristics one can obtain,(A, w) of the nonlinearity which is the ratio between S: (A-2δ1, k2δ2+krA-k1δ1-2k2δ1-2krδ1)output and the input W: (2δ2-A, k1δ1+k2δ2+2krδ2-krA) From the above points we can get both 1 and 2. With these describing function can be written as (13) It should be noted that H1 (A, w) is thetransfer function of the equivalent linearized systemof the non linearity corresponding to that particularinput amplitude A. Such transfer function is also (14) 1454 | P a g e
- 5. R.Umamaheswara rao, S.Santhosh Kumar, M.Santhi Kumar / International Journal of Engineering Research and Applications (IJERA) ISSN: 2248-9622 www.ijera.com Vol. 2, Issue4, July-August 2012, pp.1451-1458 5.1.2. LOSS MODULUS VARIATION WITH FREQUENCY 100 PLA PLA /MW C NT0.2 PLA /MW C NT0.5 PLA /MW C NT1 80 PLA /MW C NT2 Loss modulus (Mpa) 60 40 (15) 20 0 0 20 40 60 80 100 Frequency (Hz) (16) Fig.8.Frequency Vs Loss modulusWR: F=Kr*x+K1*δ1+K2*δ2 The loss module obtained from the dynamicRS: F= (Kr+K1+K2)*x+K1*δ1+K2*δ2-K1*A-K2*A frequency sweep is shown in Figure 8. DuringST: F= (Kr+K2)*x+K2*δ2-K2*A- K1*δ1 oscillatory shear flow, the total area of the interface asFrom this we can find out the damping loss factor as well as the interfacial energy is changing periodically (17) but with a much longer relaxation time than that of component polymers. It is seen that the relaxation shoulder shifts to low-frequency region with small5. RESULTS AND DISCUSSIONS addition of the MWCNTs (0.2 phr). This indicates5.1. EXPERIMENTAL RESULTS that the presence of MWCNTs retards shape5.1.1. STORAGE MODULUS VARIATION relaxation of the PLA matrix .Because the interfacialWITH FREQUENCY relaxation time is proportional to the ratio between PLA droplet size and the interfacial tension, longer 100 PLA/MWCNT0.2 PLA/MWCNT0.5 PLA/MWCNT1 interfacial relaxation process but with decreasing 80 PLA/MWCNT2 droplet size means a large decrease of interfacial storage modulus(Mpa) tension. PLA sample and the frequency dependence 60 nearly disappear. This conterminal behavior is due to formation of MWCNTs network, which highly 40 restrains the long-range relaxation of the matrix. 20 5.1.3. DAMPING LOSS FACTOR VARIATION 0 WITH FREQUENCY 0 20 40 60 80 100 Freaquency (Hz)Fig.7.Frequency Vs Storage modulus The dynamic storage moduli obtained fromthe dynamic frequency sweep are shown in Figure 7.The shoulder presented on the modulus curve of theblank PLA sample (see the arrow in Figure 7) isattributed to the shape relaxation. During oscillatoryshear flow, the total area of the interface as well as theinterfacial energy is changing periodically but with amuch longer relaxation time than that of componentpolymers. This kind of long relaxation due to thepresence of interface leads to an additional transitionshoulder on the modulus curves. It is seen that therelaxation shoulder shifts to low-frequency regionwith small addition of the MWCNTs (0.2 phr). Fig.9. Frequency Vs Damping loss factor The above graph shows damping loss factor for different nano composites. By increasing 1455 | P a g e
- 6. R.Umamaheswara rao, S.Santhosh Kumar, M.Santhi Kumar / International Journal of Engineering Research and Applications (IJERA) ISSN: 2248-9622 www.ijera.com Vol. 2, Issue4, July-August 2012, pp.1451-1458MWCNT loadings in the matrix PLA up to addition 5.1.5. VALIDATION FOR PLA/MWCNT1%of small amounts 0.2and 0.5 wt%. Further increase in SAMPLEMWCNT loadings such as 1 wt% and 2 wt% there isdecreased trend observed but these are having highdamping loss factor than matrix PLA.5.1.4. VALIDATION FOR PLA/MWCNT2%SAMPLE Fig.11.variation of theoretical and experimental loss factor for PLA/MWCNT1% sample. The above graph shows the variation of theoretical damping loss factor from the experimental damping loss factor for the sample PLA/MWCNT1. And the damping loss factor is increasing when the frequency is increased in theoretically and experimentally. In this graph there is almost a zero variationFig.10.Variation of theoretical and experimental loss we can observed and theoretical model is morefactor for PLA/MWCNT2% sample accurate in PLA/MWCNT1 than PLAMWCNT2. The above graph shows the variation of Table .2. Validation of Theoretical with experimentaltheoretical damping loss factor from the experimental results for PLA/MWCNT1%damping loss factor for the sample PLA/MWCNT2.Here the Damping loss factor is increasing when the PLA/MWCNT1 PLA/MWCNT1 %frequency is increased. (Theoretical) (Experimental) errorTable.1.Validation of Theoretical with experimental 0.139 0.142 2.1results for PLA/MWCNT2% 0.215 0.214 0 0.197 0.26 0 PLA/MWCNT2 PLAMWCNT2 % 0.399 0.43 1.4 (Theoretical) (Experimental) error 0.6031 0.62 0 0.154 0.17 9.4 10.6 0.1428 0.14 1.9 0.9105 0.92 7 0.1702 0.18 5.44 1.595 1.62 5.4 0.1362 0.39 10.43 1.81 1.83 3.6 0.502 0.54 5.66 1.875 1.9 2.2 0.81 0.9 10.88 1.39 1.43 8.53 1.5 1.52 6.88 1.77 1.8 5.38 1456 | P a g e
- 7. R.Umamaheswara rao, S.Santhosh Kumar, M.Santhi Kumar / International Journal of Engineering Research and Applications (IJERA) ISSN: 2248-9622 www.ijera.com Vol. 2, Issue4, July-August 2012, pp.1451-14585.1.6. VALIDATION FOR PLA/MWCNT0.5% 5.1.7. VALIDATION FOR PLAMWCNT0.2%SAMPLE SAMPLE Figure13. Variation of theoretical and experimental loss factor for PLA/MWCNT0.2% sampleFig.12.variation of theoretical and experimental loss The above graph shows the variation of theoreticalfactor for PLA/MWCNT0.5% sample. damping loss factor from the experimental damping loss factor for the sample PLA/MWCNT0.2%. The The above graph shows the variation of theoretical values for this sample found by usingtheoretical damping loss factor from the experimental amplitudes obtained from ANSYS for the proposeddamping loss factor for the sample PLA/MWCNT0.5. interfacial friction model. These theoretical valuesAnd the damping loss factor is increased while mainly dependent on amplitude of the specimen.increasing the frequency. In this graph there is almost a zero variation we can In this graph there is almost a zero variation observe and theoretical model is more accurate inwe can observe and theoretical model is more PLA0.2 than the other samples which are PLA2,accurate in PLA/MWCNT0.5 than both PLA1 and PLA0.5.PLAMWCNT1 and PLA/MWCNT2. Table 4: Validation of Theoretical with experimentalTable 3: Validation of Theoretical with experimental results for PLA0.2results for PLA/MWCNT0.5% PLA/MWCNT0.2 PLA/MWCNT0.2 % PLAMWCNT0.5 PLAMWCNT0.5 % (Theoretical) (Experimental) error (Theoretical) (Experimental) error 0.472 0.458 2.96 0.09873 0.1066 7.3 0.483 0.5 5.86 0.1357 0.1357 0 0.662 0.667 0 0.1926 0.18 6.5 1.073 1 9.2 0.2852 0.3 4.93 1.214 1.2 3.54 0.4694 0.5 6.12 1.1061 1 9.59 1.37 1.32 2.1 1.831 1.667 9.33 1.409 1.4 8.73 2.0752 1.857 8.4 1.802 1.8 9.2 2.0962 2.3 4.58 1.93 2 7.05 6. CONCLUSIONS From experimental results, damping loss factor increases by increasing CNT loadings up to 0.5 wt% loading of MWCNT and thereby loss factor decreases by increasing the loading of MWCNT. And also Proposed mathematical model is validated by experimental results and the maximum 1457 | P a g e
- 8. R.Umamaheswara rao, S.Santhosh Kumar, M.Santhi Kumar / International Journal of Engineering Research and Applications (IJERA) ISSN: 2248-9622 www.ijera.com Vol. 2, Issue4, July-August 2012, pp.1451-1458deviation observed from the experimental results to [13] J.Suhr, N.Koratkar, P.Keblinski, P.Ajayan,the theoretical results. Viscoelasticity in carbon nanotube With minimum error this proposed composites, Nat.Mater. 4(2005)134–137.mathematical model can be used for the extrapolation [14] H.T.Chiu, J.H.Wu, Z.J.Shong, Dynamicfor different nanocomposites. properties of rubber vibration is olatorsandanti vibration performance ofReferences nanoclay-modified PU/PEL blends system, [1] J.M.Biggerstaff, J.B.Kosmatka, Damping Polym.Eng.Sci. (2005)539–548. performance of co cured graphite/epoxy [15] R.A.Kalgaonkar,J.P.Jog,Copolyester/layered composite laminates with embedded damping silicate nanocomposites: the effect of materials, J.Compos. Mater. 33(1999)1457– molecular size and structure of the 1469. intercalantonthe structure and viscoelastic [2] J.B.Kosmatka, S.L.Liguore, Review of properties of nanocomposites, J.Polym.Sci: methods for analyzing constrained layer PartB: Polym.Phys.41 (2003)3102–3113. damping structures, J.Aerosp.Eng.6 (1993)268–283. [3] A.Baz, J.Ro, The concept and performance of active constrained layer damping treatments, J.SoundVib.28 (1994)18–21. [4] W.H.Liao, K.W.Wang, On the analysis of viscoelastic materials for active constrained layer damping treatments, J.SoundVib.207 (1997)319–334. [5] Y.Liu, K.W.Wang, Anon dimensional parametric study of enhanced active constrained layer damping treatments, J.SoundVib.223 (1999)611–644. [6] C.R.Brackbill, G.A.Lesieutre, E.C.Smith, L.E.Ruhl, Characterization and modeling of the low strain amplitude and frequency dependent behavior of elastomeric damper materials, J.Am.HelicopterSoc.45 (1) (2000)34–42. [7] A.Baz, S.Poh, Performance characteristics of the magnetic constrained layer damping, ShockVib.7 (2) (2000)81–90. [8] J.E.Lindler, N.M.Wereley, Double adjustable shockabsorbersusing electro rheological fluid, J.Intell.Mater.Syst.Struct.10 (8) (1999)652– 657. [9] G.M.Kamath, N.M.Wereley, M.R.Jolly, Characterization of magneto rheological helicopter lag dampers, J.Am.HelicopterSoc.44 (3) (1999)234–248. [10] C.L.Davis, G.Lesieutre, An active lytuned solid state vibration absorber using capacitive shunting of piezoelectric stiffness, J.SoundVib. 232(3) (2000) 601–617. [11] N.Koratkar, B.Wei, P.M.Ajayan, Carbonnanotube films for damping applications, Advanced Materials, vol.14, pp.997–1000, 2002. [12] X.Zhou, E.Shin, K.W.Wang, C.E.Bakis, Interfacial damping characteristics of carbonnanotube-based composites, Compos.Sci.Technol.64 (2004) 2425–2437. 1458 | P a g e

Full NameComment goes here.